1 Scholars' Mine Masters Theses Student Theses and Dissertations 1929 Elutriation of flotation products Guenther Walter Frotscher Follow this and additional works at: Part of the Physical Sciences and Mathematics Commons Department: Recommended Citation Frotscher, Guenther Walter, "Elutriation of flotation products" (1929). Masters Theses This thesis is brought to you by Scholars' Mine, a service of the Curtis Laws Wilson Library at Missouri University of Science and Technology. This work is protected by U. S. Copyright Law. Unauthorized use including reproduction for redistribution requires the permission of the copyright holder. For more information, please contact
2 ELUTRIATION OF FLOTATION PRODUCTS. BY GUENTHER FROTSCHER. A THESIS submitted to the faculty of the SCHOOL OF MINES AND METALLURGY OF THE UNIVERSITY OF MISSOURI in partial fulfi1ment of the work required for the Degree Of :MASTER OF SCIENCE. Rolla, Mo. May Mississippi Valley Exper~ent Station of the U.S. Bureau of liines.
3 - 1 ~ TABLE o F CONTENTS Page Preface 1 Acknowledgments 1 Purpose of Inv,estigation 2 Theory of the Elutriation Process 4 Previous Experimental Work 18 Description of the Elutriator 20 Procedure 24 A. Preparation of the Sample B. Elutrlation of the Sample...'. C. Rec'overy of the Solid Residues D. Microscopic Examination E. Chemical Analysis 32 Materials Tested 33 Discussion of Results 33 Conclusions 45 Bibliogra.phy
4 .., ii - TABLES. Page Table I. Ideal Values According to Stokes flaw. Table II. Minus 400 Mesh Material in Samples Table III. Elutriatlon of Flotation Tailings Made From a Yisaouri Dolomite Lead Ore Table IV. Screen and Elutrlation Test on Flotation Feed and Tailings From a Tri...State Zinc Ore Table V. Screen and Elutriation Test on Flotation Concentrates and Tailings From a Tenn. Zinc ore ILL U S T RAT ION S Figure 1. Elutrlation of Ground ~uartz Snnd (Ottawa) 10 Figure 2. Elutriation of Flotation Concentrate.. 17 Figure 3. Elutriator 21 Figures 4. to 13. and 15 Photomicrographs of E1utriation Products 32 a and E1utriation Feed 32 b Figure 14. Screen and Elutriation Analysis of Flotation Tailings (Uascot, Tenn.) 40 Figure 16. Elutriator ace. to Sehoene ~ 44
5 - I - PREFACE. This thesis oontains the results of an investigation carried on at the Mississippi Valley Exper~ental Station of the U.S.Bureau of Mines, Department of Com~ marce, in cooperation with the School of Mines and Metallurgy, Rolla, Mo. to study flotation products with partl~ cular reference to grain size and mineral distribution. ACKNOWLEDGKENTS. The author fs best thanks are due to J(r. W.H.Coghill, :;Jupervislng engineer, for his valuable support and to the entire staff of the Yisslssippi Valley ~per1mental Station for their kind suggestions. Furthermore he Is indebted to Mr. O.W.Ho1mes, Chemist, for his exaot ohemioal assays, to Dr. C.Y.Clayton, Professor of Metallurgy, who helped in taking photomiorographs, and to Dr. G.A.Kul1enburg, Assooiate Professor of Geology, for his aid in preparing samples for microsoopic examination. This acknowledgment would be inoomplete, if :Mr. A.Y.Gow, Assistant Metallurgist, were not mentioned, his friendly oooperation enabling the author to express himself in good English.
6 'l"'!! 2 - PURPOSE OF INVESTIGATION. Since the first application of the flotation process in ore dressing praotice, engineers have been busy solving the most delicate relations of metal distribution. in the minerals to be treated. A common method of investigating mill products is to divide the material into fractions of different grain sizes by means of a series of screens. Besides others of less importance, the well known Tyler Standard Screen Scale has been developed, in whioh the produots are soreened so that the successive sizes have a diameter of the square root of two. The number of meshes of the finest sieve has been limited by the teohnical difficulties in manufacturing with reasonable accuracy screens with very small openings. But with the development of the machinery for making very fine wire cloth, the lower ltmit of soreening has changed gradually to greater fineness. While in about 1913 an accurate 200 mesh screen could hardly be made, and 150 mesh was considered as the limit of screen analysis, within the next ten years the manufacture of 200 and 270 mesh and even of 325 mesh screens of sufficient accuracy was acoomplished. Recent~ ~ even a soreen of 400 mesh per linear inch has been made, and it has been used for this work.
7 - 3 - As a consequence of this slow development we find in the current literature most of the screen analyses done down to 200 or 325 mesh, the finest material being termed as "minus 200 mesh" or "minus 325 mesh". Little at~ tention seems to have been paid to the composition and mineral distribution within the particles of these finest materials. Further investigation of flotation concentrates is of course of little interest to the mill operator as long as his plant is running with good efficiency. When the results of concentration are insufficient, or the flow sheet must be changed for other reasons, more at" tention has to be paid to the products as regards their special composition. Examinations in this direction have shown, for example, that in the tailing from a galena flotation process the lead content generally increases with decreasing size of the slime partioles and that the product "minus 200 mesh" or "minus 325 mesh" assays highest in lead. However, on account of the lack of a suitable means of separating the material into fractions oontaining the various sized grains we are too easily inclined to consider sl~e as a definite product. Vodern technical literature contains only very few data dealing with careful examinat1onsof those products which are out of the ral1ge of ordinary screening_ Of
8 - 4 - little ~portance are notes of microscopic measurements of the particles in a minus 200 mesh sample and rough estimations of the percentages of the different grain sizes. The desire for more information was the reason for research concerning the mineral distribution in fine flotation material with particular attention to the de~ velopment of a suitable laboratory method of hydraulic classification or, as it la especially called, elutriation. THEORY o F THE ELUTRIATIOH PROCESS. Elutriation is a sizing process using an upward rising water current. While sizing by screening is dependent upon the diameter and only to a small extent upon the shape of the particles, in this process the density, shape, and size of the particles, and viscosity and temperature of the fluid are all important factors influencing more or less what is called the -hydraulic value". The hydraulic Talue 1s the rate of Tertioal flow of water expressed in cc./sec. necessary to keep the particle in suspension in a definite elutrlator; 1.e., Hydraulic Value Overflow per Second in CCt 2. Cross-Sectional Area of Elutr~ator In. cm Hence elutrlation is a method of 4ividlng finely ground products into groups each having a definite hydraulic value.
9 ~ 5 - In order to give a better picture of what hydraulio value meane and by what laws it is determined, a short discussion of the prinoiples of hydraulio classification follows. Two different conditions under which settling takes place may be distinguished: (1) Free Settling occurs where individual partioles fall freely against an opposing upward current, without being hindered by other particles. (2) Hindered Settling takes place where particles of mix~ ed sizes, shapes, and gravities in a crowded mass, yet free to move among themselves, are sorted in a rising current of water, the velocity of which is much leas than the free falling velooity of the particles, but yet enough, so that the particles are in motion. Richards, R.H., Ore Dressing McGraw~Hill Book Co, Chapter XII. Laws of Classifying by Free Settling in Water. The most ~portant factor whioh permits comparison of both laws is the terminal velocity whioh a mineral par~ ticle attains under the effect of either of the laws. The first case, free fall in water, studied first by Rittinger, oonsiders the friotion between particles and "medium to be small as compared with the dynamic effect or
10 eddying resistance of the current. The terminal velocity is expressed by the formula TO :; V 2gD(J'-1) ;; c ljd(j -1) where C is a constant depending on the charaoter of the material, D the diameter of the mineral grain, and dis the specifio gravity of the partiole. In order to find out if this formula holds for the elutriation of the material of the fineness to be discuss... ed, the equation is written as follows: c - To -~(J-l) and C is calculated for different values of D and TO. The values of TO were found by practioal elutriation of pure quartz (Ottawa) sand with a density oft!: Since C is a constant one must get, if Rittinger's theory is correct, for C an approximate constant value throughout all grain sizes. C If VDxl.65 The results of such a test gave, for 1. v o.112 mm./sec. a ," II.500 " n n =3.15 It :I 18.3
11 The resu~ts obtained show that the values for Care not oonstant, but increase with increasing hydraulic values. Therefore Rittingerts Law oannot cover the con~ ditions under which the elutriatian af such fine material takes place. The only explanation is that the particles are so fine that their classification has to be determined by the rules of "hindered settling". And indeed, the following resu~ts will prove that the law which takes into ac" oount hindered settling, covers fairly well the range of slime elutriation. This law of "viscous resistance", as it is often named, is determined oorrectly enough by Stokes' formula (unoorrected) for the terminal velocity of small roundish bodies, settling at such slow velocities, that the eddying resistance (Rittingerts Law) can be neg~ lected. Stokes' formula is as follows: 2 x g (d - 1) D 2 9xrzx4 In this formula gravity oonstant g 981 cm(sec./sec. viscosity faotor ~ =.01 gm/cm x sec. (for water at 20 0) Density of particles in gm/cm 3 diameter of particles D in om. terminal velocity To in om/sec. Since the terminal velocity and the diameters of the
12 elutriated particles are very small, we determine Din mm and get V o in mm/sea. 2 x 981 (cr- 1) D 2...'.....tIIII_ x.01 x 4 x (cf... ]. ) n 2 mm/sec D (for pure quartz) In order to find out wether or not Stokes f Law gives correct values in the range of this investigation, first of all an "ldeal A quartz sand was considered. elutriation test with metal-free The following Table I shows the ideal results. The Tyler scale was continued (approx.) below the 400 mesh limit down to 1.1 micron, and to these particle sizes, the corresponding hydraulic values were determined by Stokes' formula for a density ofrl When the results of this ideal elutriation are represented graphioally in such a manner that the logarithms of V o are plotted as ordinates against the logarithms of D as abscissae the resulting ourve must be a straight line as shown in Fig. 1. To aheek this curve by practical results an elu~ triatio. of a small sample (10 gm) of ground sand was performed. The residues were microscopically ex~ined and a representative diameter of each group determined as described previously.
13 Table I. Ideal values acoording to Stokes t Law. Mesh D in mm D2 in mm 2 va in mm/sec ' ' , ,
15 These measurements did not include the largest nor the., smallest diameters of anyone group as tests had proven that an "average" diameter is a factor too much depend... ing on the personal qualities of the observer and therefore did not check with the corresponding velooity when plotted according to Rittingerts or to Stokes' Law. But another consideration led to satisfactory results. Suppose a sample of quartz sand of a density of 2.65 was elutriated at a flow rate of, say, TO».152 mm per sec. This velocity corresponds, as shown in Table I, to a particle size of D =.013 mm. After complete elutriation at this rate, 1 0 e., after all particles smaller than.013 have been removed, and the overflow becomes perfectly clear water, the velocity is changed to the next rate, say. V o 325 mm/sec. This rate of flow corresponds to a diameter of D ~.019 mm. Now it is ObTious that the residues of this section contain all of the material larger than.013 and smaller than.019 mm.. Thus it includes grains of.0131,.0132,.0133,.0134, etc.; an innumerable number of different diameters between two limits. The prob1em resolves itself into deciding which one is the representative diameter of this group. According to Stokes it is the diameter of those partioles which a.t the oorresponding terminal velocity of the upward rising water current are kept in suspension. But it is very tmpertant to note that this holds only for
16 , perfect spheres, which never occur in the ore dressing praotice. Since the actual particles have more or less irregular forms which resist the water current more than a ball of the same hydraulic value, the diameter determined by Stokes t Law may be assumed as the diameter of that particle whioh can j~st overflow the edge of the elutriator at the oonstant terminal velocity. The practical results approve this assumption. In the report of analogous tests at the Intermountain Station of the Bureau of Mines, which will probably be published in short time, it is said in discussing Stokes' formula in connection with elutrlation: "If a value of v is taken as the velooity of the rising current, then D is the diameter of a quartz particle that will remain suspended. To overflow this partiole a stronger upward stream will be re" quired, which in turn will overflow still coarser particles that may be favorably situated. An elutriator or any classifier as a sizer leaves much to be desired, but it is the best that can be done on fine sizes. To overflow the. a certain size a some~ what stronger current is needed than indicated by Stokes! Law.-----" A table follows containing results of elutriation of a quartz sample, for each elutriation product an WaTerage size" being given. Then it is continued
17 "These results would indioate, if Stokes' Law holds, that the upward flow used was not sutt1cient~ ly strong to overflow the coarser particles in the t~e alloted, or that the fine material from the previous overflow was not thoroughly washed oui." The definition of the terminal velocity according to Stokes is given correctly in the article cited as relative velocity of the particle which will "remain in suspension n at a certain rate of flow. On the other hand, as already mentioned above, one can forego the theoretical accuracy on account of the practioal results. It was found that, when the elutriator was running, for an extremely long ttme (over night) with constant velocity, practioally no particles remained in suspension, but _the water in the cylinder became clear. This can be explained by either of two possibilities: The most probable one is that, since the mineral grains, far from being perfect spheres, often show the form of J1ate., two d~en8ions of which are large at the expense of the third one, they offer a relatively large plane to the wa.ter current and can oterflow, although their hy'drau1ic Talue would require their remaining in supen.1 There is. furthermore, a ema.1l percentage of particles odly one dimensioa otwh1oh 1s extremely large 1. comparison with the two ether ones. These grains are
18 not likely to develop suffioient resistenoe to the water ourrent and settle again on the bottom of the classifier. Another explanation for the absence of particles in suspension after long running might be that the uprising water current is very much disturbed by the rotating ~" peller' shaft resulting in higher inner friction of the particles and water, and in consequence a partial compensation of the lifting effect. These practioal considerations were the reasons for selecting the "largest" and not the "average" diameter as more nearly corresponding to Stokes t Law. The determination of an average diameter, which of course must include the largest and smallest diameters and also be based on the relative frequency of occurrence of the different sizes, proved to be too much influenced by the inaocuracies of the classifying method and by the perw sonal qualities of the.bserter. In comparing the abate: "To overflow then a certain (average) size a somewhat stronger current is needed than that indicated by Stokes' Law", with the results obtained in this investigation, which showed that the largest diameters checked well Stokes 1 foraula, it can be said that both investigations carried on independently from each other eame to the same practical corclus1on. Therefore the microscopic measurement of the quartz, and
19 - 15 ~ in consequence all other samples elutriated, included only the largest particles of eaoh section, that is to say. the largeat partioles which were present in fair percentage. To exoeedingly large grains no attention was paid since they consisted of extremely flat plates and, although their hydraulic Ta~ue agreed with that of the whole group, the dimensions were too disproportionate. The logarithms of the diameters thus obtained were plotted against the logarithms of the corresponding ve-. locities, and Fig. 1. shows that the points lie very closely to the ideal ourve calculated in Table I. Fig. 2 illustrates results of the elutriation of flotation ooncentrates of the American Zinc Co., Mascot,' Tenn. The ideal curve has been determined in the same way as for the quartz sample based on a specific gravity of the concentrates ofr! This value was ca~oulated by the method of the moisture flask. While the quartz sample was minus 200 mesh, the zinc oonoentrate sample was prepared differently. A part was left unscreened and another part was screened through 400 mesh. The course of the ourve of the unscreened concentrate shows in the larger sizes a deviation of the practical results from the ideal curte. This phen.omenon, whioh a.lrea.dy has beenobserted by' Richards, Stad1.er, amd others, inclica.tes that Stokes' Law has no
20 fllt unlimited application in this range, but Rittingerts Law does not cover accurately this interval either. We have therefore to assume that between the range covered by Stokes 1 formula v0 = K (ci' - 1) D 2 and that oovered by Rittingerfs formula v o : C (t... 1) D an intertal exists, which must be controlled by another formula. Taggart gives for this range an equation of the general form TO = c.nk where 0 and k Tary with the nature of the minerals. Taggart, A.F., Handbook of Ore Dressing, 1921, Section 6. John Wiley & Sons, New York. page 552. But as this range was out of the limit of the investigations in question BO further attention has been paid to preying or disapproting the Talid1ty of the abete formula.
22 "" PREVIOUS EXPERIMENTAL w 0 R K By no means was this the first time that fine mineral particles below the screening range were classified. Elutriation methods using different apparatus have been familiar to the ceramic engineer for many years. Good ceramic products require constituents of very uniform and, usua11y, of extreme1y fine grain size. These requirements can be met easily by using simp1e hydraulic classification. But with regard to the investigation of ore 8l~es and other fine materia1s of the ore dressing practice the research work carried on by the Bureau of Mines seeas to be one of the first of its kind. The only valuable and detailed information er earlier laboratory work in this subject was found in a Bulletin of the (English) Institution of Mining and.etallurgy. Stadler, H., Grading Analysis by Elutrlation. The Institution of' Iining and Ietallurgy, London. ' Bulleti. 104, (1913). The author of this paperdiecusses Tery comprehensite~ 1y the results'ef his elutriatio. tests with South Africa.. Rand eres. He used an elutriator similar to that seneral1y used in agri8ultural laborateries for mechanical
23 - 19..,. analysis of soils, which is known as "Schoenen...Elutriator. Since this type of elutriator wi11be taken up ~ater, a description will not be given here. Stadler was led to his elutriation work by the fact, already mentioned, that about 1.5 years ago the manufacture of an acourate 200 mesh screen was practically impossible. He therefore used as feed for the e1utriator a minus 150 mesh Rand ore. -He was oonfronted with more favorable general conditions for hydraulic classification than were those whioh determined the tests with which this paper is dealing. As it will be seen later, the diffi" culties of the elutriation increase with the increasing fineness of the material to be classified. R.H.Richards has also done work on the velocity of mineral grains falling in water; but his data are valuable only for oomparison as most of his investigations were done on coarser particles of uniform chemical composit~ ion, and details of his elutr1ation method and apparatus are not given. Richards, R.H., Ore Dressing. Second Edition Tol.I, ohapter XII, pages ; Tol.III" chapter XXXIII, pages 1420~l434. At the Intermountain Station of the Bureau of Kines in Salt Lake City, Utah, contemporary researoh wqrk on
24 - 20 t"li the same subject has been carried on. The results of this investigation were not available at the time the teats in Rolla were run. DESCRIPTION OF THE ELUTRIATOR. The original elutriator was designed a~ the Intermountain Station of the U.S.Bureau of Mines. But several changes in it were made during the course of this investigation. Its design is based on the same prin~iple as all hydraulic classifier, but the arrangement in some parts differs considerably from other elutriators. As seen in Fig.3, the elutriator consists of a vertica1 glass cylinder, 60 cm high and 50 rom inside diameter (D). The lower end is terminated by a cone. Inside the cylinder is a glass~tube shaft or rotor, on the lower end of whioh is a rubber impeller, and on the ~pper end of whioh is a bearing and a pulley. The shaft and the impeller are rotated by electric motor at 60 r.p.m. The outer diameter of the impeller shaft 1s d =18 mm. Thus the entire free area available for the upward rising water current" is A (D 2 _ d 2 )! 1710 sq.mm. 4
26 A circular overflow launder is provided on the top of the cylinder to oatch the overflowing slime. The water for the classification is stored in a zinc-lined tank of ten liters capacity. An automatic valve keeps the water lavel in the basin fairly constant by opening and closing the connection to the tap water. In order to observe occasional changes in the water level a second out" let on the tank was provided and oonnected with a vertical graduated glass tube. In contrast to other elutriators the water is introduced to the bottom of the apparatus through the shaft of the ~peller. This arrangement caused trouble during a~ost the entire period of work as it was very hard to connect the outlet of the water tank satisfaotorily with the rotating glass tube, and to furnish, at the same time, a well working regulator to keep the velooity of the water current at a constant rate for long periods of time. In the original elutriator a diaphragm valve was used for this purpose. But when the finest slimes were elutriated, i.e., when the smallest rate of water was employed, it was practically ~possible to keep the velocity constant. A regular globe TaITe, used as a substitu~e, did not work well either, and even when a s~ple olamp was applied to the rubber tubing the velocity re-
27 gulation was poor. Finally the most satisfactory control was obtained by the use of capillary glass nozzles with definite openings for the various rates of flow. An essential requirement for the successful use of these glass tips is a uniform water supply as regards cleaneness from impurities and temperature. To satisfy the first condition the tank must be built of non-cor" rosive material. Zinc proved best. A capacity of ten liters provided water of constant temperature at least for the smallest rates of flow during which the dangers from temperature variations are greatest. Of course the high fragility of the capillary glass tubes 1s disadvantageous. But the substitution of metal tubes would require the exclusive use of distilled water, since minute layers of impurities. which collect in the tips of the oapillary tubes and slowly lower the rate of flow, could not be seen. The nozzles were kept clean by washing in dilute Bulphurio acid. The following table shows the capacity of glass tubes which were used successfu11y in most of the tests,
28 Nr. Rate of Overflowing Velocity of Water in Water Cylinder cc./sec mm/sec 2..1'75 tt.102 " 3~.623 ".364 ft ft.505 tt ft " " It It " PROCEDURE. A. PR EPA RAT I O:N 0 F THE SAM P L E The preparation of a sample~.n8iated, ;first of all, in soreening as far as poss~ble. From the difficulties alread7 mentioned in handling material of extreme fineness, it might appear inadvisable to continue the screen analysis beyond, say 200 mesh, thereby producing a very fine feed for the elutrlation. At the Intermountain Station the preliminary screening was oarried on only through 200 mesh; whereas in this investigation, the elntriation feed was genera.lly a minus 400 mesh product. The reasons for this fine soreening will rellow:
29 ~ A fraction of an elutriated mill ptoduot oonsists of partioles of different sizes, depending on the specific gravity of the mineral oonstituents. Usually we will find small ore grains (galena, blende. pyrite) with larger gangue particles in the same seetion. But in an investigation of flotation products this variety in grain size is not important, since good flotation conoentrates usual~ ly contain little gangue material and good flotation tailings contain relative~y few ore particles. On the other hand poor concentrates or poor tailings contain a large percentage of particles composed of combined ore and gangue in various proportions. A sample as uniform in size as possible will b'e best fitted for the analysis by elutriation. For this purpose most of the swmples used in the teats to be discussed were size. in the Tyler scale down to 400 mesh. By this method all the material larger than.038 mm. was removed from the elutr1ator feed. Thereby also the time needed for a com.plete grading analysis was shortened, because a smaller sample gate in eaoh division Bufficient material for ohemica1 ana1ysis. The amount of materia.1 used for one run was determined by different factors. The capacity of the elutrlator and the acouraoy of the results demanded a sample as small
30 as possible. On the other hand the endeavour to de~ termlne the correct total amount of metal of eaoh overflow rate required a definite minimum of solids in each cut. These components varying with the mineralogical and structural character of the flotation produots resulted in samples of 25 to 50 gm of dry material. At first the extreme fineness of the samples caused considerable trouble by coagulation. The particles of a~ost colloidal grain size tended to unit into larger masses when agitated in water. This difficulty had to be overcome as the elutriation of flocculated material gives an absolutly wrong picture of the relations of mineral and size throughout the flotation produots. It decreases the solid material in the finest overflow in favor of the overflows of higher hydraulic values. After unsuccessful tests with alkalin hydroxides, ammonia, etc. the use of.1% solution of gum arabic proved best as a deflocculating agent. The feed sample was throughly mixed with about 300 cc. of this solution in a aeparatory funnel and left here for a.t least 12 hours. The separatory funnel permitted an easy introduction of the oonditioned sample into the cylinder of the elutriator. In general of gum arabic solution developed enough defloooulating effect for at least the first p~t of the test. A later tendenoy of oeagulation could be overcome by
31 adding a few little lumps of gum arabic in the inner glass tube without stopping the test. B. E L U T R I A T ION 0 F THE SAM P L E After conditioning the pulp in the manner described the rotor was started and the material poured into the elutriator. In order to give the mineral partlc~ les a rough pre~classificationwhile introducing the sample, a strong water flow was used in the elutriator until the glass cylinder was filled to about three-forth of its capacity. Then the water flow was reduced to its regular first (slowest) rate. By this method the finest ~articles were prevented from settling on the bottom of the elutriator below the outlet of the inner water tube. Glass beakers of two liters capacity were found satisfactory for oatohing the overflowing pulp. For the last rates where relatively small amounts of ooarse material were carried over by large quantities of water t bigger vessels such as enamel pane and buckets are better fitted. In general it can be stated that the time required for a complete elutriation test depends chiefly upon the velocity of the water flow at the start, since the first rate of flow takes the greatest percentage of the entire time of the run. When starting with a velocity of.035 mm.
32 - 28 ""' per sec. which equals an overflow of.06 cc. per sec. the time for elutriating a 25 gm sample of minus 400 mesh material requires from 8 to 12 hours, the first rate of overflow taking 40 to 60% of this time. The physical composition of the product had a greater effect upon the time than the weight of the material tested (25 or 50 gm). c. R E C 0 V E R Y o F THE SOL I D RESIDUES. Gum arabic, although favorable as a dispersing agent, was disagreeable in its effect after the elutriation was finished. It was found impossible to settle out completely the solid particles from the overflow if smallest hydraulic value. The finest material, less than 5 microns in diameter, remained partly in suspension. It was found that from this first overflow after a settling t~e of about one day, 90 to 95% of the solida settled out, the amount differing somewhat with the character of the product, while the rest remained in suspension even after several days. Since the finest particles are often the most important, and since even for large tonnages of mi11 products only 25 gin are taken as a sample, it is neoessary to recover as much as possibleo! the suspended solids and te reduoe 108ses to a min~um. In order to do this many of the ge-
33 till! 29 - nerally known coagulating agents were tried. Some acids seemed to be good flocculators~ but as their maximum efficiency is dependent on a very definite concentration with respect to the amount of solids, a factor extremely variable in an elutriated overflow, none of these coagulating reagents proved as satisfactory as might be ex~ pected. A relatively simple means of bringing the solid particles out of suspension was finally found in the centrifuge. The advantage of this apparatus is that the concentration of the suspensi~n~ the reagents used for dispersion, and the hydrogen ion concentration play very little part. A practio~1ly complete separation of two liters of suspension containing mostly minus 5 micron material could be accomplished in an eleotric centrifuge of 2400 r.p.m. speed with four 50 cc. glass tubes in about 2 1/2 hours. This time could be shortened by using the centrifuge with a crown for larger tubes. Before centrifuging the suspensions of the finest overflows the losses of residues amountea as high as 7 to 9% by weight. This was cut down by the use of the centrifuge to about 1 to 1.5%. A small loss in this very fine size seems to be unavoidable, and is chiefly due to the dir.. I. f1cu1ty of completely removing the dried solids from the beakers. Even by very careful use of a soft brush the for-
34 mation of dust is hardly avoidable, and a oertain amount of material oannot be recovered at all because of its hygroscopic behaviour. In some cases it was found advisable to wash out the finest material with a small amount of alcohol, which was afterwards evaporated. At the Intermountain Station where also gum arabic is being used as dispersing agent, a good precipitating effeat has been found in the addition of copper sulphate and ammonia to the suspension. The copper hydrate preci~ pitate formed carries down all dispersed material and is then dissolved in Hydrochloric acid. After the clear water had been poured out of the settled beakers, or the suspension had been centrifuged, the solid residues were dried. Here again it proved advantageous to have used but the minimum amount of gum arabic for conditioning the pulp before the elutriation. A large amount of this electrolyte in the residues tended to form dark brown crusts on. the bottom of the vessel thus rendering a complete recovery of the solids more difficult o D. M I era S COP I C EXAMINATION. The microscopic examination was carried on with a regular metallurgical microscope using an eye~ piece micrometer and transmitted light. It consisted of single measurements of six different grains in a repre-
35 sentative sample of each fraotion. The mean value was taken as the representative diameter of the product. No attention was paid to particles two diameters of which were greatly different. Some difficulty arose in measuring the finest elutriated overflow because the minute particles of the highly hygroscopic powder were hard to separate on the slide. A1cohol was used as a dispersing agent. In certain cases the conditioning of the sample with a solution of Canada balsam in xylol similar to that suggested by SchneiderhOhn. proved best. Schneiderhohn, H., Anleitung zur mikroskopischen Besttmmung und Untersuohung von ~zen und Aufbereitungsprodukten besonders tm auffallenden Licht. Berlin page 61. The photomicrographs, Fig.4 to 11, show fairly well the uniformity in grain size of various elutriation products, which is in striking contrast to the irregularity of grain size in the unelutriated minus 400 mesh products, Fig.12 and 13. The samples are Tri-State flotation tailings, except in Fig.ll and 15, which show Ottawa. quartz and-south East Missouri dolomite. The hydraulic values represented by the photomioro- gra.phs are:
36 Fig. 4 above 3.22 co./eee. (residue in spigot) n tt... It " " ".. It 8.50 n 9.18 n n " " " E. C HEM I CAL ANALYSIS. The dry residues were weighed and assayed. The chemical analysis is the deciding factor in determining the size of the sample to be graded. When the produets are low in metal content about two gm of dry residue is needed for each assay. When the metal content is exceedingly low, still lar$er fractions are required. The Mascot flotation tailings assayed in the composite sample only 0.092% Zn and required at least 5 gm of solids in each portion for exact results. This necessitated using a large elutriation sample. On the other hand samples of one gm were sufficient in the ease of elutriated concentra.tes.
39 MATERIALS TES TED. In as muoh as other experimental work was being done on mill produots from the South East Missouri Lead Eelt and the Tri~State Zinc District flotation products from these distriots were tested by elutriation. In ad~ dition crushed (Ottawa) quartz sand in the fundamental tests and flotation products from Mascot, Tenn. were also elutriated. In one case flotation tailings which were produced in the laboratory were tested in order t. show the changes in mineral distribution by improved flotation method. DIS C U S S ION o F RESULTS. The results of teats are shown in the acoompanying tables. Table II illustrates the results of screening various preducts through the 400 mesh screen. (page 34) From this table it can be seen that the minus 400 mesh part of flotation tailings assays higher in metal than the tota1 tailings, and oonsequently higher tha~ the plus 400 mesh part. For concentrates the opposite is true: The plus 400 mesh fraction assays higher than the minus 400 mesh fraction. Elutriation enables separations to be made far beyond the 400 mesh point. The results of complete grading tests. t
40 are given in the Tables III, IV, and V. Table II. Minus 400 Mesh Material in Samples. Total Per Cent Per Cent Metal in Per Cent Name of Product Wei~ht Metal in - in Complete -400 Mesh 400 ]lesh Sample Product Product Bonne Terre Flat.Tails Pb.125 Pb 81.9 Tri-State " Zn 1.94 Zn 59.1 " " Feed Zn 6.19 Zn 42.2 It Lab. " Tails Zn.'77 Zn 55.9 tmasaot Flotation " Zn..15 Zn 53.2 " " Cone Zn Zn 27.1
41 "" 35 - Table III. Elutriation Test of Flotation Tailings Made From a Missouri Dolomite Lead Ore. Per Cent Assay Per Per Cent Grain Size Weight Cent Lead Total Lead Mesh Mesh " " " n " " " " + 25 Microns Mi.r t " 5 " " ~
42 Table IV. Screen and E1utriation Test an Flotation Feed and Tailings from a Tri-State Zinc Ore.." + Gra.in Size ;eer Cent Weight Weed Assay Per Cent Zn Per Cent Total Zn ][111 Lab. Feed Mill Lab. Feed Mill Lab. Tailings Tailings Tailings 48 Mesh «, ft " " n " ' Microns It " Ilol 5 " Total tloo.o a..oo.o :"
43 TableV. Screen and Elutriation Test on Flotation Concentrates and Tailings from a Tennessee Zinc Ore. Per Cent Weight Assay Per Cent Zn Per Cent Total Zn Grain Size Concentr. Tails Concentr. Tails Concentr. Tails + 35 Mesh Mesh " It ~ It ~ n " , " ~4bO'" 35 Microns I " ~.5 I It I- l5~ 10 n :3 " 6.4, ~ 3 n Total
44 - ;5a - When we oompare the results given in the Tables III, IV, and V it is striking that the sections on the boundary between screening and elutriation assay high in metal. That indicates that the coarsest elutriation product, or the last overflow from the elutriator, representing in general but a small percentage by weight, is very rich in metal. This oan be explained by the fact that a commercial hydraulic classifier usually alao gives a relatively rich product in the first spigot, which classifies with the highest velocity of the water current, if a pre-screened material is fed. In this product of highest hydraulic value the differenc between screen classification and grading by elutrlation is greatest. The following consideration shows the mechanical explanation. In considering a complete series of elutriation products of a mill sample we find in eaoh section of equal hydraulic value two different types of particles: Relatively large gangue particles and relatively small ore partioles. Screening the sample before elutriation through a definite soreen means "therefore removing a part of the large gangue particles from the group of highest hydraulic value. Consequently the last overflow product of any elutrlation the feed ()~ which has been soreened will assay high
45 in metal. It should alao be noted that the minus 5 micron fractions of the tailings assay highest in metal and contain the largest percentages of the total metal of all the fractions. In contrast,' the minus 10 micron fraction of the concentrates is relatively low in metal content and carries only a small amount of the total metal. The example, given may be slightly exaggerated since coagulation and incomplete separation reduced the amount of the finest material reoovired. In F1g.l4 the results of a complete size analysis including screening and elutriation is plotted in the cumulative percentages. The values obtained in the practica.l test form two faily regular ourves. A small irregularity can be noted in the transition zone between finest screening and coarsest elutriation products where, as explained above, the differenoe between screening and elutriation is particularly great. In considering the results it can be stated that the elutriator as developed in the course of these tests gives good results which are in general free from objeotions. There can be of course different opinions as to the accura~ cy required for' the purpose in question. On all procedures where by skill and oareful manipulations avoidable inaccu~ racy can be eliminated, the utmost care must be maintained. However there are som.e inherent errors based on the
47 - 41 "" special construction of the elutriator used whioh cannot be avoided, but can be reduced to a minimum. The whole series of tests haa shown that a ohief source of trouble is the introduction of the water through the rotating shaft of the impeller. Here two factors oannot be brought into agreement. They are (1) to provide between the end of the inner glass tube and the bottom of the elutriator a space wide enough to make possible elutriation of the coarsest particles, and (2) at the a~e time to have the space as small as possible to force the water current through the lowest layers of the s~ple to be classified. It could be seen from the report of the experimental work at the Intermountain Station that this arrangement did not work very satisfactorly in those intestigations e1ther J but the effect was probably not so great as in the tests at Rolla, where elutriation was done on samples of minus 400 mesh f1neness in 6 or 7 steps as c~pared with minus 200 mesh material graded in 3 steps in Salt Lake City. Furthermore the ratio of the diameter of the elutriator cylinder to that of the impeller shaft does not yet seem to be right. The ratio of the present arrangement is 50:18, i.e. the diameter of the cylinder is not yet three times as large as that of the smaller tube. Observations on the running elutriator showed that the
48 "" relatively big inner tube causes the upward rising current to form whirl:poo~s resulting in inaccurate classification of the sample. This trouble oan probably be reduoed by either increasing the di~eter of the elutriator cylinder or by decreasing that of the ~:pel1er shaft or better by changing both diameters respectively. The difficulties in maintaining a water current con~ stant for long time at slow rate had been mentioned in the description of the elutriator. Perhaps some other type of water feeder can be designed to give more satisfactory regulation. Considering all these diffioulties it is appearent that the statement that the apparatus gives good results does n~t hold unless utmost care and watch are used, a condition that may be called burdensome and uneconomic with regard to the long time required for each te~t. Here the author cannot help asking if net a classifier of less complioated type would giye the same, maybe better, results while less supervision is required. The tests Stadler has reported on were performed in an elutriatorwhich is known as Schoene-Elutriator". On this desigm the mechanism for stirring up the sample is entir.1y missing. That ie possible as the water current enters the classifier en the lowest point of the cone through a. gla.ss cock from without. This arrangement pro-
49 ~ 43 - vides an uniformily rising current t which cannot be disturbed by mechanical agitation of any kind. Since Stadler does not mention any difficulties in regulating a constant flow, this trouble seems also to be overcome. He used for changing the rates of flow in steps oonstant for all tests a piezometer,. the arrangement of which can be seen from the sketch inclosed (Fig.16). Stadler says as regards uniformity of the smallest velocity of the classifying water current: ItThe displacement of the finest slime takes a long time, but as the level in the piezometer keeps extremely steady the apparatus can safely be left, and other work undertaken in the meantime." As there was no chance of trying an elutriator of the tppe Stadler used for his tests the design of an elutriator as suggested in Fig. 16 will be open to cri"" ticism. But it seems probable that at least three factors which caused much trouble and inaccuracy in the present arrangement, call be Lmproved if not absolutely eliminated. They are (1) The introduction of the water on the lowest point of the elutriator results in classifying the entire sample without leaving a sma11 layer of unclassified materia1 in the cone of the olassifier.
51 (2) Omission of mechanically moved parts provides an undisturbed water current (except unavoidable friotion on the walls of the cylinderl (3) A well lubricated glass cock cooperating with the piezometer gives a chance of easy regulation of the same and constant rates of flow for any tests. CON C L U S ION S as ~egards In summarizing the results of this research ita usefulness for general flotation practice special attention might be paid to the fact that in all flotation tailings the highest percentage of the total metal content was found oonnected to the finest particles, minus 5 microns in fineness. In flotation concentrates the total amount of metal in this size range is relatively small. This phenomenon leads to the statement that the efficiency of flotation methods is limited by a lower particle size, below which the concentrate recovery decreases rapidly. Comparatively few of the minus 5 microns metal-bearing particles are recovered as flotation concentrates, most of them go into tailings. This observation justifies the tendency of modern
52 flotation practice of avoiding as far as possible any over-grinding.
53 ~ BIBLIOGRAPHY. Taggart, A.F., Handbook of Ore Dressing, ~ohn Wiley & Sons, New York. Richards, R.H., Ore DTessing, McGraw-Hill Book Co., New York. Stadler, H. Grading Analysis by E1utriation. The Institution of Mining & Metallurgy, Bulletin 104. (1913). London. Schneiderhohn, H., Anleitung zur mikroskopischen Bestimmung von Erzen und Aufbereitungepro..., dukten besonders 1m auffallenden Lichte. Berlin _.. _--~-_.-
Apr 17, 2000 LAB MANUAL 1302.0 1302 PARTICLE SIZE ANALYSIS OF SOILS AASHTO Designation T 88 (Mn/DOT Modified) 1302.1 SCOPE This method describes a procedure for the quantitative determination of the distribution
Test Procedure for PARTICLE SIZE ANALYSIS OF SOILS TxDOT Designation: Tex-110-E Effective Date: August 1999 1. SCOPE 1.1 This method covers the quantitative determination of the distribution of particle
Math Matters: Dissecting Hydrometer Calculations By Jonathan Sirianni, Laboratory Assessor In the 16th century Galileo and the Tower of Pisa made famous the fact that two objects, no matter their mass,
Viscosity It is the property of a liquid due to which it flows in the form of layers and each layer opposes the motion of its adjacent layer. Cause of viscosity Consider two neighboring liquid layers A
Chemistry 112 Laboratory Experiment 6: The Reaction of Aluminum and Zinc with Hydrochloric Acid Introduction Many metals react with acids to form hydrogen gas. In this experiment, you will use the reactions
EXPERIMENT 10 PERMEABILITY (HYDRAULIC CONDUCTIVITY) TEST CONSTANT HEAD METHOD 106 Purpose: The purpose of this test is to determine the permeability (hydraulic conductivity) of a sandy soil by the constant
CONSTANT HEAD AND FALLING HEAD PERMEABILITY TEST 1 Permeability is a measure of the ease in which water can flow through a soil volume. It is one of the most important geotechnical parameters. However,
Experiment 12- Classification of Matter Experiment Matter can be classified into two groups: mixtures and pure substances. Mixtures are the most common form of matter and consist of mixtures of pure substances.
METHOD A10 (a) THE DETERMINATION OF THE IN-PLACE DRY DENSITY OF SOIL OR GRAVEL BY THE SAND REPLACEMENT METHOD 1 SCOPE The in-place dry density of compacted soil or gravel, as defined below, is determined
GRADATION OF AGGREGATE FOR CONCRETE BLOCK Although numerous papers have been written concerning the proper gradation for concrete mixes, they have generally dealt with plastic mixes, and very little published
1 Grain Size Distribution Sieve Analysis The University of Toledo Soil Mechanics Laboratory Introduction The grain size distribution is a representation of the approximate distribution of soil grain sizes
September 1, 2003 CONCRETE MANUAL 5-694.200 5-694.210 PROPERTIES OF CONCRETE PROPERTIES AND MIX DESIGNATIONS 5-694.200 Inspectors should familiarize themselves with the most important properties of concrete:
THE SOLUBILITY OF A SALT IN WATER AT VARIOUS TEMPERATURES 2007, 1995, 1991 by David A. Katz. All rights reserved. Permission for academic use provided the original copyright is included. OBJECTIVE To measure
130 Experiment-366 F MEASUREMENT OF VISCOSITY OF LIQUIDS BY THE STOKE S METHOD Jeethendra Kumar P K, Ajeya PadmaJeeth and Santhosh K KamalJeeth Instrumentation & Service Unit, No-610, Tata Nagar, Bengaluru-560092.
DRINKING WATER - LAB EXPERIMENTS LAB EXPERIMENTS Coagulation and flocculation Jartest coagulation and flocculation - jartest lab experiments Framework This module explains the lab experiment on coagulation
SIEVE ANALYSIS OF FINE AND COARSE AGGREGATES FOP FOR AASHTO T 27 (11) MATERIALS FINER THAN 75 µm (No. 200) SIEVE IN MINERAL AGGREGATE BY WASHING FOP FOR AASHTO T 11 (11) Scope Sieve analysis determines
CENTRIFUGAL PUMP SELECTION, SIZING, AND INTERPRETATION OF PERFORMANCE CURVES 4.0 PUMP CLASSES Pumps may be classified in two general types, dynamic and positive displacement. Positive displacement pumps
Test Procedure for SIEVE ANALYSIS OF FINE AND COARSE AGGREGATES TxDOT Designation: Tex-200-F Effective Date: January 2016 1. SCOPE 1.1 Use this test method to determine the particle size distribution of
PERMEABILITY TEST A. CONSTANT HEAD OBJECTIVE To determine the coefficient of permeability of a soil using constant head method. need and Scope The knowledge of this property is much useful in solving problems
SODIUM CARBOXYMETHYL CELLULOSE Prepared at the 28th JECFA (1984), published in FNP 31/2 (1984) and in FNP 52 (1992). Metals and arsenic specifications revised at the 55 th JECFA (2000). An ADI not specified
EXPERIMENT 4: Separation of a Mixture of Solids Read the entire experiment and organize time, materials, and work space before beginning. Remember to review the safety sections and wear goggles when appropriate.
TECHNICAL DATA SHEET Duro hard chrome plating process is a high-speed bath which employs a special mixed soluble catalyst and has been developed to meet the modern hard chrome plating requirements. Its
September 1, 2003 CONCRETE MANUAL 5-694.300 MIX DESIGN 5-694.300 NOTE: FOR PROJECTS REQUIRING CONTRACTOR MIX DESIGN, THE DESIGN PROCEDURES ARE SPECIFIED IN THE SPECIAL PROVISIONS OF THE CONTRACT. 5-694.301
Factors Affecting Precipitation of Calcium Carbonate John A. Wojtowicz Chemcon Laboratory tests with clear solutions showed that precipitation of calcium carbonate does not occur in the ph range 7.5 to
Recovery of Elemental Copper from Copper (II) Nitrate Objectives: Challenge: Students should be able to - recognize evidence(s) of a chemical change - convert word equations into formula equations - perform
SHIBAYAMA SCIENTIFIC CO., LTD. DENSITY MEASURING SYSTEMS Density Gradient Tube Method Direct Reading Type A / Type B Comply with the standards below: JIS K-0061-1992, K-7112 1980 ASTM D1505 Type A /Left
1 Experiment 7: Titration of an Antacid Objective: In this experiment, you will standardize a solution of base using the analytical technique known as titration. Using this standardized solution, you will
Reaction of Magnesium with Hydrochloric Acid (Gas Laws) Your Name: Date: Partner(s) Names: Objectives: React magnesium metal with hydrochloric acid, collecting the hydrogen over water. Calculate the grams
Identification of a Substance by Physical Properties 2009 by David A. Katz. All rights reserved. Permission for academic use provided the original copyright is included Every substance has a unique set
EML 316L Experiment 3 Pipe Friction Laboratory Manual Mechanical and Materials Engineering Department College of Engineering FLORIDA INTERNATIONAL UNIVERSITY Nomenclature Symbol Description Unit A cross-sectional
Florida Method of Test for TESTING OF GROUND TIRE RUBBER Designation: FM 5-559 1 SCOPE 1.1 This method is used to determine the physical requirements of ground tire rubber for use in asphalt rubber using
Experiment 8, page 1 Version of April 25, 216 Experiment 446.8 SIZE OF A MOLECULE FROM A VISCOSITY MEASUREMENT Theory Viscous Flow. Fluids attempt to minimize flow gradients by exerting a frictional force,
PURPOSE: To verify a proposed mechanism for the hydrolysis of t-butyl Chloride. PRINCIPLES: Once the Rate Law for a reaction has been experimentally established the next step is its explanation in terms
ENE 806, Project Report 3 CHEMICAL PRECIPITATION: WATER SOFTENING Grégoire Seyrig Wenqian Shan College of Engineering, Michigan State University Spring 2007 ABSTRACT The groundwater with high level initial
EXPERIMENT #8 Name: PRE-LABORATORY ASSIGNMENT: Lab Section 1. The alkali metals are so reactive that they react directly with water in the absence of acid. For example, potassium reacts with water as follows:
COMMON LABORATORY APPARATUS Beakers are useful as a reaction container or to hold liquid or solid samples. They are also used to catch liquids from titrations and filtrates from filtering operations. Bunsen
Experiment 3 Separation by Solvent Extraction Objectives To separate a mixture consisting of a carboxylic acid and a neutral compound by using solvent extraction techniques. Introduction Frequently, organic
Millikan Oil Drop Experiment Matthew Norton, Jurasits Christopher, Heyduck William, Nick Chumbley Norton 0 Norton 1 Abstract The charge of an electron can be experimentally measured by observing an oil
Filter Aid Filtration Filtration is the separation of solids from liquids by forcing the liquid to flow through a porous medium and depositing the solids on the medium. A filter aid (finely divided material
SOME USES OF SPRAY NOZZLES It is important that the nozzle you select is appropriate for your particular application Liquid sprays are used in a seemingly endless variety of applications Some of the more
www.swagelok.com Valve Sizing Te chnic al Bulletin Scope Valve size often is described by the nominal size of the end connections, but a more important measure is the flow that the valve can provide. And
RHEOLOGY RHEOLOGY Science describing the flow and deformation of matter under stress. Rheo = the flow Viscosity (η) is the resistance of a fluid material to flow under stress. The higher the viscosity,
STP 206-1 Standard Test Procedures Manual Section: 1. SCOPE 1.1. Description of Test 2. APPARATUS This method describes the procedure for determining the relationship between the particle size distribution
CENTRIFUGAL PUMP OVERVIEW Presented by Matt Prosoli Of Pumps Plus Inc. 1 Centrifugal Pump- Definition Centrifugal Pump can be defined as a mechanical device used to transfer liquid of various types. As
INVESTIGATION OF FALLING BALL VISCOMETRY AND ITS ACCURACY GROUP R1 Evelyn Chou, Julia Glaser, Bella Goyal, Sherri Wykosky ABSTRACT: A falling ball viscometer and its associated equations were studied in
105 Adopted: 27.07.95 OECD GUIDELINE FOR THE TESTING OF CHEMICALS Adopted by the Council on 27 th July 1995 Water Solubility INTRODUCTION 1. This guideline is a revised version of the original Guideline
Chapter 5 Using Newton s Laws: Friction, Circular Motion, Drag Forces Units of Chapter 5 Applications of Newton s Laws Involving Friction Uniform Circular Motion Kinematics Dynamics of Uniform Circular
Spectrophotometry and the Beer-Lambert Law: An Important Analytical Technique in Chemistry Jon H. Hardesty, PhD and Bassam Attili, PhD Collin College Department of Chemistry Introduction: In the last lab
SOLUBILITY OF A SALT IN WATER AT VARIOUS TEMPERATURES LAB Purpose: Most ionic compounds are considered by chemists to be salts and many of these are water soluble. In this lab, you will determine the solubility,
81 experiment5 LECTURE AND LAB SKILLS EMPHASIZED Synthesizing an organic substance. Understanding and applying the concept of limiting reagents. Determining percent yield. Learning how to perform a vacuum
Molysulfide Particle Size Analysis INTRODUCTION Molysulfide is the Climax Molybdenum Company trade name for lubricant grade molybdenum disulfide (MoS 2 ). The mineral designation for MoS 2 is Molybdenite
Linings Linings Along with technical and metallurgical advancement in piping materials, research on lining requirements for pipe and fittings has resulted in the development of linings to meet many different
Test Procedure for SOIL-LIME TESTING TxDOT Designation: Tex-121-E Effective Date: August 2002 1. SCOPE 1.1 This method consists of three parts. 1.1.1 Part I determines the unconfined compressive strength
RECALL FIRST CLASS: Q K Head Difference Area Distance between Heads Q 0.01 cm 0.19 m 6cm 0.75cm 1 liter 86400sec 1.17 liter ~ 1 liter sec 0.63 m 1000cm 3 day day day constant head 0.4 m 0.1 m FINE SAND
The Basic Principles of Sieve Analysis Introduction Many natural and manufactured materials occur in a disperse form, which means that they consist of differently shaped and sized particles. The particle
8.9 - Flash Column Chromatography Guide Overview: Flash column chromatography is a quick and (usually) easy way to separate complex mixtures of compounds. We will be performing relatively large scale separations
AN EXPERIMENT IN ALCHEMY: COPPER TO SILVER TO GOLD 2005, 2000, 1996 by David A. Katz. All rights reserved INTRODUCTION One of the goals of the ancient alchemists was to convert base metals into gold. Although
General Physics Lab: Atwood s Machine Introduction One may study Newton s second law using a device known as Atwood s machine, shown below. It consists of a pulley and two hanging masses. The difference
Using a pot model to represent osmosis Student sheet To do 1 Set up the potato investigation as instructed. 2 Record the mass of the potato which is then placed in distilled water... g 3 Record the mass
#3. Acid - Base Titrations 27 EXPERIMENT 3. ACID-BASE TITRATIONS: DETERMINATION OF CARBONATE BY TITRATION WITH HYDROCHLORIC ACID BACKGROUND Carbonate Equilibria In this experiment a solution of hydrochloric
Physical and Chemical Properties and Changes An understanding of material things requires an understanding of the physical and chemical characteristics of matter. A few planned experiments can help you
EXPERIMENT 7 Reaction Stoichiometry and Percent Yield INTRODUCTION Stoichiometry calculations are about calculating the amounts of substances that react and form in a chemical reaction. The word stoichiometry
Chemistry 119: Experiment 1 The Analytical Balance Operation of the Single-Pan Analytical Balance Receive instruction from your teaching assistant concerning the proper operation of the Sartorius BP 210S
STP 206-4 Standard Test Procedures Manual Section: 1. SCOPE 1.1. Description of Test This method describes the procedure for determining the liquid limit, plastic limit and the plasticity index of coarse-grained
Phosphate Recovery from Municipal Wastewater through Crystallization of Calcium Phosphate A. Alamdari, Ph.D. * and S. Rohani, M.Sc. * Department of Chemical Engineering, School of Engineering, Shiraz University,
Carbon Dioxide and an Argon + Nitrogen Mixture Measurement of C p /C v for Argon, Nitrogen, Stephen Lucas 05/11/10 Measurement of C p /C v for Argon, Nitrogen, Carbon Dioxide and an Argon + Nitrogen Mixture
CHEMICAL REACTIONS OF COPPER AND PERCENT YIELD Objective To gain familiarity with basic laboratory procedures, some chemistry of a typical transition element, and the concept of percent yield. Apparatus
HEATING AND POURING To perform a casting operation, the metal must be heated to a temperature somewhat above its melting point and then poured into the mold cavity to solidify. In this section, we consider
1) Error Analysis Apparatus Errors (uncertainty) Every time you make a measurement with a piece of apparatus, there is a small margin of error (i.e. uncertainty) in that measurement due to the apparatus
SEPARATION OF A MIXTURE OF SUBSTANCES LAB Purpose: Every chemical has a set of defined physical properties, and when combined they present a unique fingerprint for that chemical. When chemicals are present
(adapted from Blackburn et al., Laboratory Manual to Accompany World of Chemistry, 2 nd ed., (1996) Saunders College Publishing: Fort Worth) Purpose: To prepare a sample of soap and to examine its properties.
Volumetric Analysis Lecture 5 Experiment 9 in Beran page 109 Prelab = Page 115 Experimental Aims To prepare and standardize (determine concentration) a NaOH solution Using your standardized NaOH calculate
Chemistry 12 IB Corrosion of Iron Rajesh Swaminathan March 13, 2005 1 Planning A 1.1 Aim The aim of the experiment is to investigate factors that affect the rate of corrosion of iron. More specifically,
1 P age Module 7: Hydraulic Design of Sewers and Storm Water Drains Lecture 7 : Hydraulic Design of Sewers and Storm Water Drains 2 P age 7.1 General Consideration Generally, sewers are laid at steeper
WD-DWGB-3-4 2009 Corrosivity of Water Supplies What is meant by Corrosivity? Corrosive water can be defined as a condition of water quality which will dissolve metals from metallic plumbing at an excessive
Pump ED 101 Positive Displacement Pumps Part I Reciprocating Pumps Joe Evans, Ph.D http://www.pumped101.com There are many pump designs that fall into the positive displacement category but, for the most
Geotechnical Measurements and Explorations Prof. Nihar Ranjan Patra Department of Civil Engineering Indian Institute of Technology, Kanpur Lecture No. # 28 Last lecture we have covered this Atterberg limit,
ELECTRIC FIELD LINES AND EQUIPOTENTIAL SURFACES The purpose of this lab session is to experimentally investigate the relation between electric field lines of force and equipotential surfaces in two dimensions.
Laboratory Testing Manual Date: 99 06 21 Page 1 of 7 METHOD OF TEST FOR DETERMINATION OF PERMEABILITY OF GRANULAR SOILS 1. SCOPE 1.1 This method covers the determination of the coefficient of permeability
Lapping and Polishing Basics Applications Laboratory Report 54 Lapping and Polishing 1.0: Introduction Lapping and polishing is a process by which material is precisely removed from a workpiece (or specimen)
Practical Student sheet Practical : Wear eye protection. Ensure the delivery tube does not become blocked. Ethanoic acid will sting if it gets into cuts in the skin. Equipment boiling tube stand and clamp
The Effect of Spring Pressure on Carbon Brush Wear Rate Jeff D. Koenitzer, P.E. Milwaukee, Wisconsin, USA Preface 2008 For decades there was extensive testing of countless different carbon brush contact
University of California at Santa Cruz Jack Baskin School of Engineering Electrical Engineering Department EE-145L: Properties of Materials Laboratory Lab 5b: Temperature Dependence of Semiconductor Conductivity
MATHEMATICS: THE LEVEL DESCRIPTIONS In mathematics, there are four attainment targets: using and applying mathematics; number and algebra; shape, space and measures, and handling data. Attainment target